Standard Practices for Measurement of Liquidus Temperature of Glass by the Gradient Furnace Method
The liquidus temperature is the maximum temperature where equilibrium exists between the amorphous glass and its primary crystalline phase. A sample of about 30 gm is crushed to -20 mesh and placed in a platinum boat with dimensions of 0.5" x 0.5" x 6.0". The glass specimen is held at a specified temperature gradient over its entire length for a period of time necessary to obtain thermal equilibrium between the crystalline and glassy phases. The specimen is quenched and viewed with a microscope to determine the glass/crystalline interface location and corresponding temperature.
SIGNIFICANCE AND USE
These practices are useful for determining the maximum temperature at which crystallization will form in a glass, and a minimum temperature at which a glass can be held, for extended periods of time, without crystal formation and growth.
1.1 These practices cover procedures for determining the liquidus temperature (Note 1) of a glass (Note 1) by establishing the boundary temperature for the first crystalline compound, when the glass specimen is held at a specified temperature gradient over its entire length for a period of time necessary to obtain thermal equilibrium between the crystalline and glassy phases.
Note 1-These terms are defined in Terminology C162.
1.2 Two methods are included, differing in the type of sample, apparatus, procedure for positioning the sample, and measurement of temperature gradient in the furnace. Both methods have comparable precision. Method B is preferred for very fluid glasses because it minimizes thermal and mechanical mixing effects.
1.2.1 Method A employs a trough-type platinum container (tray) in which finely screened glass particles are fused into a thin lath configuration defined by the trough.
1.2.2 Method B employs a perforated platinum tray on which larger screened particles are positioned one per hole on the plate and are therefore melted separately from each other.
1.3 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use.
Extracted, with permission, from ASTM C829 Standard Practices for Measurement of Liquidus Temperature of Glass by the Gradient Furnace Method, copyright ASTM International, 100 Barr Harbor Drive, West Conshohocken, PA 19428. A copy of the standard may be purchased from ASTM International, phone 610-832-9555, e-mail: email@example.com, website: www.astm.org.
FROM THE BLOG...
Measuring Flexural Creep of Ceramic Investment Casting Shells Understanding the creep behavior...
5 Ceramic Products That Changed the World! When you think of ceramics, many people may flash...
01/22/2018Orton Welcomes New General Manager!
The Board of Trustees of the Edward Orton Jr. Ceramic Foundation announces the retirement of its General...